O De La Barrière

C Appino

C Ragusa

F Fiorillo

M Lobue

F Mazaleyrat

D and 2D loss measuring methods: optimized setup design, advanced testing, results

Keywords: Magnetic losses, Magnetic measurements, Permeameter, Two-dimensional magnetization

Accurate measurements of magnetic losses in laminations are a prerequisite for their theoretical assessment, as well as for satisfying calculations of energy dissipation in engineering systems. The standardized and universally applied measurement method, used as a reference for the definition of the material quality in the specification standards, is based on the Epstein test frame magnetizer. Its success relies on the reproducibility of the performed measurements. Its limitations come, on the one hand, from cumbersome sample preparation and, on the other hand, from a certain divergence of the measured loss figures from the true loss figures. Similar systematic differences between measured and true loss values are also observed with the standard Single Sheet Tester method. In both cases, measurements under bi-dimensional induction are or cannot be envisaged. The design of new measurement setups and magnetizers overcoming the drawbacks of the Epstein and Single Sheet Tester methods and possibly becoming recognized Standards in the future is welcome, but challenging. This paper is devoted to a comprehensive discussion of the state of the art in the alternating and two-dimensional measurements of energy losses in soft magnetic materials for electrical applications. We will summarize, in particular, measuring solutions proposed in the current literature and we will discuss in detail recent developments achieved in the authors' labs regarding 1D measurements with compensated permeameters and 2D measurements at high inductions and high frequencies.

I. INTRODUCTION

lectrical machine designers are nowadays facing difficult challenges. For example, the rapid growth of demand in embedded applications, such as hybrid/electric cars [1], require the design of very compact actuators [START_REF] Hua | Investigation and design of a high-power flux-switching permanent magnet machine for hybrid electric vehicles[END_REF]. In this context, materials are often used at the limit of their thermal viability, so realistic designs impose accurate loss calculations. Should these be based on magnetic loss models or should they rely on empirical formulations, there is no alternative to precise loss measurements [START_REF] Kowal | Comparison of iron loss models for electrical machines with different frequency domain and time domain methods for excess loss prediction[END_REF]. The standard measurement methods, based on the use of the Epstein frame [4] [5] or the Single Sheet Testing (SST) magnetizer with flux closing yokes [6], offer good reproducibility, as verified by a number of international comparisons [START_REF] Sievert | Magnetic measurements on electrical steels using Epstein and SST methods[END_REF] [START_REF] Appino | International comparison on SST and Epstein measurements in grain-oriented Fe-Si sheet steel[END_REF]. They are therefore assumed as reference methods for the definition of the material quality in the specification standards. However, both Epstein and SST methods generate systematic contributions to the measurement uncertainty [START_REF] Fiorillo | Measurement and characterization of magnetic materials[END_REF] and the obtained loss figures can be appreciably different from the "true" loss values, those provided by accurate local measurements of the effective magnetic field strength and the flux density [START_REF] Appino | International comparison on SST and Epstein measurements in grain-oriented Fe-Si sheet steel[END_REF] [9] [START_REF] Ferrara | Effective versus standard Epstein loss figure in Fe-Si sheets[END_REF]. An example concerning non-oriented and grain-oriented Fe-Si steel sheets is shown in Fig. 1. It is to remark that the Epstein strip samples require tedious preparation, including relief of cutting stresses. In addition, Epstein and SST methods are hardly compatible with two-dimensional induction loci [START_REF] Sasaki | Measurement of rotational power losses in silicon-iron sheets using wattmeter method[END_REF], a typical working regime in electrical machine cores. It turns out that the losses due to the two components of the flux density locus are often computed separately and summed up, as if they were independent alternating magnetization processes [START_REF] Abou-Elyazied Abdallh | A Non-Destructive Methodology for Estimating the Magnetic Material Properties of an Asynchronous Motor[END_REF]. This procedure is clearly inaccurate, especially at high flux density values, where the hysteresis loss, always increasing with alternating flux, tends to vanish under circular flux density on approaching the saturation. No measuring standards exist for rotating flux density, though many research efforts have been devoted to the development of 2D induction setups. Different solutions have actually been envisaged for the 2D magnetizer, like the horizontal [START_REF] Enokizono | Rotational power loss of silicon steel sheet[END_REF][14] [START_REF] Makaveev | Accurate field strength measurement in rotational single sheet testers[END_REF] and vertical [START_REF] Nencib | 2D analysis of rotational loss tester[END_REF] [START_REF] Enokizono | Magnetic field analysis of rotational loss tester with vertical yoke[END_REF] cross-shaped yokes and the three-phase yoke with either hexagonal [START_REF] Hasenzagl | Novel 3-phase excited single sheet tester for rotational magnetization[END_REF] or circular [START_REF] Appino | Loss decomposition under two-dimensional flux loci in non-oriented steel sheets[END_REF] samples. In the latter case, flux density values up to 1.85 T could be reached, with maximum frequency around a few hundred Hz, under both alternating and rotational flux [START_REF] Appino | One-dimensional/two-dimensional loss measurements up to high inductions[END_REF]. These limiting values of flux density and frequency should however be overcome, in order to meet the conditions of modern electrical machine cores, often attaining the saturated state and working at kHz frequencies.

In this paper, present-day developments in alternating and two-dimensional measurements of magnetic losses will be discussed, with emphasis on recent progress made in the authors labs (SATIE, INRIM, Politecnico di Torino), overcoming the previous limits. Two main points are addressed: -Alternating flux. The Single Sheet Tester will be specifically considered, because it allows for a flexible approach to material testing. SST measurements may show slightly inferior reproducibility with respect to the Epstein measurements [START_REF] Appino | International comparison on SST and Epstein measurements in grain-oriented Fe-Si sheet steel[END_REF], since the quality of the yoke, its losses, and the reluctance of the sheet-yoke contact region can play a role. A novel approach to the SST method [START_REF] De La Barriere | A simple compensation method for the accurate measurement of magnetic losses with a single strip tester[END_REF], where the potential drop occurring in different parts of the magnetic circuit is automatically compensated by means of a feedback system, will be here highlighted. -Two-dimensional flux. The ambitious objective of reaching very high flux density values and high frequencies under controlled 2D fluxes and measuring the associated loss figures has been addressed in recent times (see for example [START_REF] Gorican | 2-D measurements of magnetic properties using a round RSST[END_REF] or [START_REF] Appino | Alternating and Rotational Losses up to Magnetic Saturation in Non-Oriented Steel Sheets[END_REF]). To this end, two setups have been realized, those employ circular samples and three-phase magnetizers. One setup has been optimized to reach the kilohertz range, the other for approaching the magnetic saturation. Both fieldmetric and thermometric loss measurement methods have been applied. Significant results for rotating and alternating flux densities will be discussed in the following.

II. LOSS MEASUREMENTS UNDER ALTERNATING MAGNETIC FIELD STRENGTH

A. Standard methods

The characterization of soft magnetic materials under alternating magnetic field strengths is well standardized, but room exists for improved and wider-range measurements. We summarize here the main features of the present-day measuring approaches.

1) Toroidal sample.

Measurements in soft magnets can seldom be done on open samples, because demagnetizing fields are large and generally non-uniform. But a perfectly closed magnetic circuit, free of macroscopic demagnetizing effects, can ideally be achieved only using toroidal samples with uniformly distributed primary winding [START_REF] Fiorillo | Measurement and characterization of magnetic materials[END_REF]. This approach is widely used with bulk materials, such as ferrites and Soft Magnetic Composites (SMC) [START_REF] De La Barrière | Loss separation in soft magnetic composites[END_REF], and described in the standards [25] [26]. It can be used with materials in sheet or ribbon form, either tapewound or made by stacking punched rings, possibly after release of bending or residual stresses by annealing. Problems nevertheless arise, because, with the length of the circumferential magnetic field strength lines depending on the inverse of their diameter, a ratio between outer and inner diameter Do / Di < 1.1 is prescribed, a condition sometimes difficult to fulfill [START_REF] Zurek | Prediction of power loss and permeability with the use of an artificial neural network in wound toroidal cores[END_REF]. Limitations may also appear regarding the maximum number of turns, that is, the maximum applicable magnetic field strength value .

2) Epstein frame

The Epstein frame is adopted in the IEC60404-2 standard for measurements on magnetic sheets. These are cut as strip samples (length 300 mm, width 30 mm), stacked and arranged to form a square magnetic circuit with double lapped joints. The related IEC standards cover the frequency ranges DC  f  400 Hz (700-turn primary and secondary windings) [4] and 400 Hz  f  10 kHz (200-turn windings) [5]. A fixed magnetic path length lm = 0.94 m is assumed, independently of material, flux density level, and frequency. Non-oriented (NO) alloys are tested by stacking alternate layers of strips cut along the rolling direction (RD) and the transverse direction (TD), in order to cope with the non-negligible anisotropic response of these materials. The properties of the grain-oriented (GO) alloys are instead measured on strips cut along the rolling direction. A main advantage of the Epstein frame is the good reproducibility of the measurements, as verified by international comparisons [7] [8]. Fig. 2 provides an example of dispersion of results concerning the measurement of the 50 Hz power losses PEpst and PSST in GO steels, as obtained by eleven different laboratories belonging to academia and industry [START_REF] Appino | International comparison on SST and Epstein measurements in grain-oriented Fe-Si sheet steel[END_REF]. The statistical analysis is made on 212 loss figures (after excluding few outliers) provided by the participating laboratories. The data concern five different GO steel types, tested at the peak polarization values Jp = 1.3, 1.5, 1.5, 1.7 T. The global relative standard deviation of the measured PEpst values around the best estimate <P> is Epst = 0. 82 % (SST = 0. 88 %). Since the very same samples are tested and the stacking procedure is strictly defined, the dispersion among the laboratories best estimates is attributed to the performance and the calibration features of the measuring setups.

The imperfections (capacitive effects, leakage flux…) of the Epstein frame that can affect the loss measurements have been discussed by Brugel, et al. [START_REF] Brugel | Effects of the Epstein Frame imperfections on the accuracy of power measurements at medium frequencies[END_REF]. By assuming a defined magnetic path length lm = 0.94 m one makes an obvious oversimplification, inevitably conflicting with the evolution of the flux patterns in the magnetic circuit with f, Jp, and the material type. We can nevertheless lump the objective complexity of such an evolution into an effective magnetic path length leff(Jp), associated with the effective (true) power loss value Peff, which relates then to lm and the standard Epstein loss figure PEpst according to

) ( / ) ( ) ( p eff m p epst p eff J l l J P J P   (1)
The results in Fig. 1 are therefore understood in terms of monotonical increase of leff(Jp) with Jp, both in NO and GO sheets. Fig. 3. Two Epstein frames with different limb lengths have been employed to determine the effective magnetic path length leff(Jp). Its derivation relies on the assumption that the power loss in the corner regions is independent of the frame size [START_REF] Marketos | A method for defining the mean path length of the Epstein frame[END_REF] [START_REF] Qingyi | Determination of the weighted mean path length of the Epstein frame[END_REF]. The problem of justifying from a physical viewpoint the behavior of leff(Jp) has been considered both through Finite Element calculations [START_REF] Antonelli | Epstein frame: How and when it can be really representative about the magnetic behavior of laminated magnetic steels[END_REF] and by ad hoc experiments. Ahlers and Sievert compared Epstein frame and single strip measurements and justified the found behavior of leff by expressing it as leff = l0 + (l/2c)lc, the sum of the legs length l0 and a portion of the corners length lc depending on the ratio of the leg to corner permeabilities l and c [START_REF] Ahlers | Comparison of a single strip tester and Epstein frame measurements[END_REF]. A natural approach to the determination of leff consists in assuming, as done in [START_REF] Marketos | A method for defining the mean path length of the Epstein frame[END_REF] [START_REF] Qingyi | Determination of the weighted mean path length of the Epstein frame[END_REF], that the total power loss Epst measured with the Epstein frame can be decomposed in two terms, one (l0) in the limbs, the portion of the frame of length l0 covered by the windings, the other (c) in the corners . The somewhat crude assumption is made in [START_REF] Marketos | A method for defining the mean path length of the Epstein frame[END_REF][30] that c is independent of the frame size and the polarization is uniform in the limbs, thereby making l0 proportional to the limbs length. By comparing the loss figures obtained with two frames having different limb length, the two loss contributions are discriminated. A standard 25 cm frame and a reduced 17.5 cm frame have been considered in [START_REF] Marketos | A method for defining the mean path length of the Epstein frame[END_REF] [START_REF] Qingyi | Determination of the weighted mean path length of the Epstein frame[END_REF], as sketched in Fig. 3. If the total loss values Epst1 andEpst2 are measured in the larger and smaller frame, respectively, we can write

) ( ) ( ) ( ) ( ) ( ) ( p 2 p c p Epst2 p 1 p c p Epst1 J Π J Π J Π J Π J Π J Π l l     (2)
and we obtain

) ( ) ( ) ( ) ( p 2 p 1 p Epst2 p Epst1 J Π J Π J Π J Π l l   
. In this way, the loss per unit volume

    0 0 / l p l p p PJ Π J Al  ,
where A is the cross-sectional area of the sample, is obtained and the effective magnetic path length is retrieved from (1). A similar approach has been followed by the authors of [START_REF] Parent | Determination of Specific Losses in the Limbs of an Epstein Frame Using a Three Epstein Frame Methodology Applied to Grain Oriented Electrical Steels[END_REF], who used three Epstein frames. However, small deviations from uniformity of the magnetization inside the Epstein legs inevitably occur, impairing to some extent this conclusion. A detailed investigation on the evolution of effective magnetic field strength and polarization along the limbs, performed by means of localized H-and B-coils, on non-oriented, conventional grain-oriented (CGO) and high-permeability grain-oriented (HGO) sheets, actually shows non-negligible decrease of the polarization value Jp(x) across the limb length from center to corners in all materials [START_REF] Ferrara | Effective versus standard Epstein loss figure in Fe-Si sheets[END_REF]. Fig. 4 provides an example of decrease of Jp(x) across the Epstein limbs in NO Fe-Si strips. If

dx x J l J l l ) ( 1 2 / 2 / p 0 0p 0 0   
is the peak polarization value measured by the secondary Epstein winding, the conventional power loss figure is obtained as

dt t J t i l N T J P T ) cos( ) ( 1 ) ( 0p 0 H m H 0p epst       (3)
where iH(t) is the magnetizing current. The corresponding true power loss is given by the average value of the locally measured power loss Peff(x) across the length l0

dx x J P l J P l l )) ( ( 1 ) ( p 2 / 2 / eff 0 0p eff 0 0    (4)
The power loss increases more than linearly with Jp, according to the power law Peff(Jp)  Jp n , with n, in turn, a function of Jp. Peff(J0p) becomes then dependent on the profile of Jp(x) and the effective magnetic path length will consequently evolve with J0p according to the equation

) ( ) ( ) ( 0p eff 0p epst m 0p eff J P J P l J l   ( 5
)
leff is found to be an increasing function of J0p in all the previous NO (0.5 T  J0p  1.5 T) and GO (1.0 T  J0p  1.8 T) alloys. It approximately ranges between 0.92 m and 0.98 m. Such an increase is understood and calculated in terms of Jp(x) profile and n(Jp) behavior [START_REF] Ferrara | Effective versus standard Epstein loss figure in Fe-Si sheets[END_REF].

3) Single Sheet Tester (SST) Fig. 5. The loss figure measured with the SST method PSST (IEC60404-3) in CGO and HGO alloys is higher (1 % -5 %) than the same quantity (PEpst) measured using the Epstein frame (IEC60404-2) (adapted from [START_REF] Appino | International comparison on SST and Epstein measurements in grain-oriented Fe-Si sheet steel[END_REF], where the symbol <.> means the mean result between the different laboratories of the international comparison).

The SST standard IEC 60404-3 is based on the use of a single sheet of length 500 mm and width ranging between 300 mm and 500 mm, inserted between the pole faces of a double-C 500 mm  500 mm flux-closing laminated yoke, made of GO Fe-Si sheets [6] [START_REF] Sievert | The measurement of magnetic properties of electrical sheet steel-survey on methods and situation of standards[END_REF]. Primary and secondary windings are uniformly distributed on a former surrounding the sheet and the magnetic field strength is derived from the measured magnetizing current and Ampère's law, assuming a fixed magnetic path length lm = 0.450 m. Thanks to the large width of the test sample, edge effects are negligible and hardening due to sample cutting can be disregarded. It is a remarkable advantage of SST with respect to the Epstein method, where stress relief annealing of the cut strips is usually required [START_REF] Klimczyk | Influence of cutting techniques on magnetostriction under stress of grain oriented electrical steel[END_REF] [START_REF] Loisos | Effect of mechanical and Nd: YAG laser cutting on magnetic flux distribution near the cut edge of non-oriented steels[END_REF]. SST testing of laser-scribed GO Fe-Si can, for example, be directly performed on the treated sheets. Epstein strips should instead be annealed before scribing, in order to keep the beneficial effect of the local deformation by the scratch lines on the domain structure. On the other hand, SST and Epstein methods show comparable reproducibility features, although SST may be more prone to outlying results, ensuing from imperfections, residual magnetism, and loss in the yokes [37] [38]. Again, the fixed magnetic path length is conducive to a systematic deviation of PSST(Jp) from Peff(Jp), different from and difficult to reconcile with PEpst(Jp) through simple formulation. It is found, in general, that PSST(Jp) > PEpst(Jp), as illustrated for a number of CGO and HGO sheets in Fig. 5.

The typical solution adopted for overcoming the drawbacks associated with the IEC60404-3 standard consists in directly measuring the effective magnetic field strength at the sample surface by means of an H-coil. Since this is somewhat impractical with the 500 mm wide sheets, downsized fixtures with strip samples large enough (e.g. 60 mm) to avoid effects from workhardened edges, have been proposed [START_REF] Miyagi | Development of measurement system of magnetic properties at high flux density using novel single-sheet tester[END_REF] [START_REF] Nakata | Analysis of magnetic fields in a single sheet tester using an H coil[END_REF]. H-coil measurements are not easy, because a rigid multiturn thin sensor must be realized and accurately calibrated [START_REF] Fiorillo | A reference system for the measurement of low-strength magnetic flux density[END_REF][42] and the induced signal at power frequencies can be very small and noisy, besides requiring integration. This makes this method appropriate for precise measurements in the laboratory, but unsuitable for the industrial practice. Use of Ampère's law, where the magnetic field strength value is retrieved from the magnetizing current, > FOR CONFERENCE-RELATED PAPERS, REPLACE THIS LINE WITH YOUR SESSION NUMBER, E.G., AB-02 (DOUBLE-CLICK HERE) < 6 without incurring in the systematic uncertainty associated with the definition of the magnetic path length in IEC 60404-3 or the difficult handling of H-coil low signals, would require some efficient compensation method. By this, we could neutralize the interference of the yokes on the determination of the loss figure, while maintaining zero magnetic potential drop. The classical compensated DC permeameters, like the Burrows [START_REF] Svala | An improved, practical Burrows permeameter[END_REF] and the Iliovici [START_REF] Barranger | Very high temperature permeameter[END_REF] permeameters are based on the idea of compensating the drop of magnetomotive force (MMF) occurring in the flux-closing yoke by supplying and suitably adjusting the current flowing in auxiliary windings adjacent to the yoke pole faces. A modern version of AC SST compensated permeameter, discussed in [START_REF] Nafalski | Loss measurements on amorphous materials using a fieldcompensated single-strip tester[END_REF], is based on the idea of using a Chattock coil, placed upon a defined central portion of length lm of the sheet sample as a zero signal indicator. The sample is inserted between the pole faces of a double-C laminated yoke and the auxiliary windings are supplied via a high-gain amplifier by the signal generated in the Chattock coil. With magnetizing solenoid and sample suitably longer than lm, near-zero Chattock signal can be maintained, which implies uniform tangential magnetic field strength over the magnetic path length lm. A weak point of the Chattock coil method consists in the difficulty of handling the very low signal generated by the coil. We have recently demonstrated that the MMF can actually be controlled with high sensitivity on a defined length of the sample, without using a sensor [START_REF] De La Barriere | A simple compensation method for the accurate measurement of magnetic losses with a single strip tester[END_REF]. Such a control is exerted by means of auxiliary windings located on the yoke branches, as sketched in Fig. 6. It works in such a way that the magnetic path length becomes

B. A novel approach to the compensated SST permeameter.

L =190 mm l L =290 mm o +
exactly equal to the distance L1 between the pole faces of the yoke. To this end, the upper yoke is endowed with sharp wedgeshaped pole faces, whose tip lines are in contact with the sample sheet at the precise distance L1. By imposing that the MMF drop along the upper yoke is zero, one obtains a magnetic path length coincident with L1, according to the reluctance scheme shown in Fig. 6b. We denote here by RS, RY, and RP the reluctance of the sample sheet, the lower and upper yokes, and the wedge-shaped poles, respectively. The auxiliary winding on the lower yoke generates the MMF NcIc, which is controlled in such a way as to cancel the flux circulating in the upper yoke. The PID controller on the feedback loop keeps in fact the voltage V1 = d1/dt detected on the upper yoke vanishingly small by supplying via a high-gain amplifier a magnetizing current to the winding on the lower yoke, where all the flux is eventually deviated. Since the flux in the upper yoke is zero, wedge-shaped bulk poles are perfectly appropriate. The adopted magnetic field strength value H = Ni/L1, for a current i circulating in the exciting N-turn solenoid, is compared with the effective magnetic field strength value, obtained by integrating the voltage simultaneously detected by a many-turn flat H-coil placed on the sample surface. By using the yoke itself as a zero MMF indicator, we obtain much larger signal than achievable with the Chattock coil, with ensuing easier and more precise control around the zero value. Fig. 7. Energy loss W and apparent power S are measured in GO steel sheets using the newly developed permeameter with and without compensation and with the H-coil method. The measurements are made at 100 Hz as a function of the peak polarization Jp. Compensation leads to drastic reduction of the discrepancies existing between the results obtained with the uncompensated permeameter and the H-coil method.

An example of loss measured at f = 100 Hz by the magnetizing current method, with and without compensation, as a function of peak polarization Jp on GO Fe-Si 30 mm wide strips is given in Fig. 7a. A 50 mm  50 mm cross-sectional area permeameter is used. The measured loss figures are compared with those obtained by the H-coil method. The discrepancy between the results provided by the compensated permeameter and the H-coil measurements is lower than 1 % beyond Jp = 0.75 T, that is, within the typical measuring uncertainty of the SST method [START_REF] Appino | International comparison on SST and Epstein measurements in grain-oriented Fe-Si sheet steel[END_REF]. A similar comparison for the apparent power is provided in Fig. 7b.

In summary, the merits of this new type of compensated permeameter can be stated as follows: 1) The loss and apparent power figures are close to the ones measured with the H-coil method; 2) The results are independent of the yoke properties and the reproducibility of the loss figures is in principle ensured, though high permeability GO sheets in the yoke manufacture are recommended for good sensitivity; 3) The effective magnetic field strength is obtained by measurement of the magnetizing current (no need for treating small signals); 4) Only slight modification of standard SST setups is required; 5) This method remains effective at very low frequencies, for which the H-coil method becomes too noisy to get reliable results.

III. TWO-DIMENSIONAL MAGNETIZATION MEASUREMENTS: SETUPS AND RESULTS

A. Measurement setups

The characterization of soft magnetic sheets under two-dimensional flux has a long story, going back to the end of the 19 th century [START_REF] Baily | The hysteresis of iron and steel in a rotating magnetic field[END_REF]. The interest in this type of measurements has chiefly to do with the study of the energy losses in rotating machines [START_REF] Moses | Importance of rotational losses in rotating machines and transformers[END_REF] and three-phase power transformers [START_REF] Pfutzner | Rotational magnetization in transformer cores: A review[END_REF][49] [START_REF] Moghadam | Comparison of flux distribution in three-phase transformer cores assembled from amorphous material and grain oriented silicon iron[END_REF]. A survey of the measurements setups and arising problems are given in the recent book [START_REF] Zurek | Characterisation of soft magnetic materials under rotational magnetisation[END_REF]. No standards exist for 2D magnetic measurements and a variety of measuring methods are in use [START_REF] Fiorillo | Measurement and characterization of magnetic materials[END_REF]. This fact, in conjunction with a certain experimental complexity, is the main reason for the substantial discrepancies found in the results from different laboratories [START_REF] Sievert | European intercomparison of measurements of rotational power loss in electrical sheet steel[END_REF] [START_REF] Ragusa | An intercomparison of rotational loss measurements in non-oriented Fe-Si alloys[END_REF]. In early attempts to measure the 2D magnetic losses, either cross-shaped samples with orthogonal pickup coils [START_REF] Kaplan | Magnetic core losses resulting from a rotating flux[END_REF] [START_REF] Moses | Measurement of rotating flux in silicon iron laminations[END_REF] or disk samples placed at the center of two perpendicular rectangular Helmholtz pairs coils supplying a maximum magnetic field strength around 20 kA/m [START_REF] Strattant | Iron losses in elliptically rotating fields[END_REF], were tested. Nowadays, the Rotational Single Sheet Testers (RSST), of either vertical or horizontal type, are typically employed. The vertical RSST derives from the standard SST magnetizer for alternating flux density, to which an orthogonal second double-C yoke is added [START_REF] Nencib | Performance evaluation of a large rotational single sheet tester[END_REF][58], as sketched in Fig. 8. The magnetizing coils are wound around the yokes and a large sheet sample is generally used, in order to achieve good magnetic field strength homogeneity in the measuring region, typically located at the center of the sample.

The horizontal RSST is realized as a cross-shaped laminated magnetizer with a gap, inside which a square sheet sample is placed [START_REF] Zouzou | Magnetic properties under unidirectional and rotational field[END_REF] [60] [61] [START_REF] Enokizono | Rotational power loss of silicon steel sheet[END_REF]. It is verified that a square sample ensures better magnetic field strength homogeneity than a circular one [START_REF] Xu | On the reproducibility, standardization aspects and error sources of the fieldmetric method for the determination of 2D magnetic properties of electrical sheet steel[END_REF], much more so if the yoke laminations are stacked perpendicular to the sample plane, thereby hindering flux leakage between the adjacent salient poles [START_REF] Enokizono | Numerical analysis of accuracy of rotational magnetic loss measurement apparatus[END_REF] [START_REF] Zurek | Digital feedback controlled RSST system[END_REF]. Acceptably good flux homogeneity is actually obtained upon a relatively small region across the sample center [START_REF] Nencib | 2D analysis of rotational loss tester[END_REF] and modifications of the salient poles, supported by Finite Element calculations, have been realized for the sake of widening such a region [START_REF] Zhu | Measurement and modelling of losses under two dimensional excitation in rotating electrical machines[END_REF] [START_REF] Makaveev | Accurate field strength measurement in rotational single sheet testers[END_REF].

Improved homogeneity of the magnetic flux is obtained by adopting a circular sample inserted in the stator core of a rotating machine [START_REF] Ragusa | An intercomparison of rotational loss measurements in non-oriented Fe-Si alloys[END_REF][19] [START_REF] Gorican | 2-D measurements of magnetic properties using a round RSST[END_REF], either two-phase or three-phase. A variant of this approach consists in using an hexagonal sample inside a three-phase magnetizer [START_REF] Pfutzner | Rotational magnetization in transformer cores: A review[END_REF] [START_REF] Hasenzagl | Novel 3-phase excited single sheet tester for rotational magnetization[END_REF]. The three-phase choice ensures a power advantage in supplying the 2D magnetic field strength (three power amplifiers can be used instead of two) and the flexibility of an additional degree of freedom in the control of the flux loci [START_REF] Appino | Loss decomposition under two-dimensional flux loci in non-oriented steel sheets[END_REF]. The price to pay is a certain complexity of the feedback algorithm, requiring a matrix transformation before the conventional fixed point iteration scheme [START_REF] Ragusa | A three-phase single sheet tester with digital control of flux loci based on the contraction mapping principle[END_REF]. Relatively sophisticated control methods, based on adaptive correction algorithms [START_REF] Zurek | Use of novel adaptive digital feedback for magnetic measurements under controlled magnetizing conditions[END_REF], can be found in literature. Other authors prefer simpler methods, even if a non-negligible number of iterations might be required [START_REF] Zurek | Practical implementation of universal digital feedback for characterisation of soft magnetic materials under controlled AC waveforms[END_REF]. Another interesting variant is the system presented in [START_REF] Alatawneh | Design of a novel test fixture to measure rotational core losses in machine laminations[END_REF]. The rotating flux density is generated by a system of electromagnets working as an array of Halbach magnets. Good homogeneity of the flux density can be reached by such a system.

Recently, 3D magnetizers have been developed, for the specific objective of testing bulk Soft Magnetic Composites (SMC). They are obtained by arranging C-shaped yokes along three orthogonal planes, by which cubic samples can be tested with flux loci lying on a generic plane [START_REF] Li | Study on Rotational Hysteresis and Core Loss Under Three-Dimensional Magnetization[END_REF].

B. Measurement of 2D magnetic losses

The measurement of the magnetic losses under a rotating magnetic field strength is typically accomplished on open samples. Consequently, magnetizing current and effective magnetic field strength are in a complex relationship and an H-coil is preferably used to determine the magnetic field strength on the measuring area. With the additional knowledge of the local flux density and the usual integration of their product, the loss figure is obtained. This is the rule for 2D loss measurement, but it is in some cases associated with or substituted by the thermometric method [START_REF] Strattant | Iron losses in elliptically rotating fields[END_REF], where the increase of the sample temperature upon energy dissipation is measured.

If

dt t V NA t H dt t V NA t H ) ( ) ( 1 ) ( ) ( ) ( 1 ) ( Hx y 0 y Hx x 0 x         (6)
where (NA)x and (NA)y are the turn-area products of the coils. With uniform flux density in the measuring area, tangential (Hx(t), Hy(t)) and effective magnetic field strength components coincide and associate with the components (Bx, By). These are typically obtained by threading a couple of few-turn windings through small (0.5-0.75 mm) holes drilled symmetrically on the measuring region, as illustrated for a disk sample in Fig. 9b. The flux density components are then calculated from the detected e.m.f.s (VBx(t),VBy(t)), according to

        x Bx Bx x y By By y 1 1 B t V t dt NA B t V t dt NA       (7)
where NBx and NBy are the number of turns of the B-windings, and (Ax, Ay) are the linked cross-sectional areas of the material. To avoid drilling the sample and the possible perturbations induced by this process (which can in any case be removed by annealing), the needle method, where point-like contacts are made in place of holes and the related voltage drop is detected, has been implemented [73][74]. The detected signal, however, is generally very low and noisy, and this method is not in general use.

The precise measurement of (Bx(t),By(t)) requires the accurate determination of the cross-sectional areas (Ax, Ay) linked with the B-windings. Given the rounded profile of the holes, the geometrical determination of (Ax, Ay) in the sheet samples can be inaccurate. In addition, on approaching very high polarization values, precise correction for the air-flux is required, but the actual turn-area of the B-coils is not accurately known. For its precise determination, the saturation polarization of the material is first measured by a standard method (e.g., using a permeameter) on a conventional strip sample with well-known cross-sectional area. The disk sample is then inserted between the pole faces of a Type-B permeameter ( [START_REF] Fiorillo | Measurement and characterization of magnetic materials[END_REF], pp. 311) and the flux x = NBx(JAx+0HAt), where J is the polarization and At is the total area (air plus sample) linked with the Bx winding, is measured. The effective magnetic field strength H, measured at the coil position by means of a Hall plate, is increased beyond about 150 kA/m, thereby ensuring full magnetic saturation J = Js. The linear increase of x versus H is exclusively due to the term 0HAt in highmagnetic field strength region. We obtain in this way the area At and, for any sufficiently high magnetic field strength H0, the measuring cross-sectional area of the sheet sample

  x 0 Bx 0 0 t x Bx S H N H A A NJ     (8)
The reason of this procedure is to solve the uncertainty on the section introduced by the holes diameter. By repeating the same procedure along the y-direction, Ay is obtained and the loss can finally be calculated from the measured magnetic field strength and flux density components and their time dependence according to the Poynting theorem y x x y 0 ( )

T dB dB W H H dt dt dt   [J/m 3 ] (9)
To remark here the inevitable approximation involved with the measurement of the effective magnetic field strength in the open sample, with its large and relatively inhomogeneous demagnetizing field. The H-coil provides, because of its finite thickness, an overestimate of the true magnetic field strength value in the sample. This fact, however, does not interfere with the loss measurement, because true and measured magnetic field strengths differ by a quantity proportional to the magnetization.

A further drawback of the fieldmetric 2D loss measurement can derive from possible slight misalignment and imperfect orthogonality of the H-and B-windings [START_REF] Gorican | Unreliable determination of vector B in 2-D SST[END_REF] [76] [START_REF] Sievert | Studies on the measurement of two dimensional magnetic phenomena in electrical sheet steel at PTB[END_REF]. This leads to different loss values when measured with the magnetic field strength rotating clockwise (CW) or counterclockwise (CCW). While the difference is reduced, though not negligibly [START_REF] Zurek | Effect of off-axis H-coil sensitivity on clockwise-anticlockwise differences of rotational power loss in isotropic samples[END_REF], at low flux density values, dramatic divergence between CW and CCW rotational losses can be observed at high flux densities (e.g., beyond 1.5 T in non-oriented alloys) [78] [79]. This discrepancy can be largely, though not fully, compensated by averaging the results of the CW and CCW measurements [START_REF] Todaka | Counterclockwise/clockwise (CCW/CW) rotational losses under high magnetic field[END_REF][81] [START_REF] Zurek | On the difference between clockwise and anticlockwise power losses, Part 1: Mathematical study[END_REF], as the geometrical phase lag is reversed relatively to the electromagnetic phase lag.

At high flux densities, the phase shift between flux density and magnetic field strength (actually, its fundamental harmonic) may become too small to be measured with sufficient accuracy. Consequently, the thermometric method, where the magnetic power loss is associated with the rate of heating of the sample, would rather be used rather than the usual fieldmetric method. In > FOR CONFERENCE-RELATED PAPERS, REPLACE THIS LINE WITH YOUR SESSION NUMBER, E.G., AB-02 (DOUBLE-CLICK HERE) < 11 the ideal case of adiabatic measurements on a material of specific heat cp, the power loss per unit mass is related to the time derivative of the temperature according to

dt dT c P / p   [W/kg] ( 10
)
The temperature is measured either with a thermocouple stuck on the sheet surface [START_REF] Fiorillo | Measurement and characterization of magnetic materials[END_REF][57] or a thermistor [START_REF] Albir | Improved dc bridge method employed to measure local power loss in electrical steels and amorphous materials[END_REF]. Good agreement between the fieldmetric method and the thermocouple-based thermometric method is verified in NO steel sheets [START_REF] Appino | One-dimensional/two-dimensional loss measurements up to high inductions[END_REF]. The thermistor sensors actually appear better suited to localized loss investigations, as those concerning high-permeability widedomains GO steels [START_REF] Albir | Improved dc bridge method employed to measure local power loss in electrical steels and amorphous materials[END_REF]. The relative complexity of the 2D measurements, due to the open sample configuration, the related need for bulky magnetizers, and the relatively awkward control of the flux loci, have traditionally limitated the range of frequency and flux density Bp. This becomes apparent when the reported capabilities of the main laboratories dealing with the 2D characterization of nonoriented steel sheets are considered and compared, as shown in the peak flux density versus test frequency map shown in Fig. 10. The maximum experimental frequency is typically around a few hundred Hz and reliable results are hardly obtained beyond 1.7 T -1.8 T [START_REF] Zurek | On the difference between clockwise and anticlockwise power losses, Part 1: Mathematical study[END_REF]. The reported 2D measuring limits regard INRIM (before year 2010) [START_REF] Appino | Loss decomposition under two-dimensional flux loci in non-oriented steel sheets[END_REF] [START_REF] Appino | One-dimensional/two-dimensional loss measurements up to high inductions[END_REF], Wolfson Centre WCM [START_REF] Zurek | Rotational power losses and vector loci under controlled high flux density and magnetic field in electrical steel sheets[END_REF], G2ELAB Grenoble [START_REF] Spornic | Frequency magnetic behaviour of SiFe sheets in a rotational field[END_REF][85], PTB Braunschweig [START_REF] Maeda | An evaluation method of cross-type H-coil angle for accurate two-dimensional vector magnetic measurement[END_REF], Gifu Univ. [START_REF] Mori | 2-D magnetic rotational loss of electrical steel at high magnetic flux density[END_REF]. Actually, present-day high-speed rotating machines involve frequencies in the kHz range [START_REF] Sulaiman | Design of 12-slot 10-pole Permanant Magnet Flux-Switching Machine with hybrid excitation for hybrid electric vehicle[END_REF]), and mass reduction requirements force machine designers to deal with flux density levels around 2 T, as highlighted in Fig. 10. The dashed line in this figure, covering such (Bp, f) limiting profile, reflects the enhanced 2D measuring capabilities recently attained by the joint efforts of the SATIE/INRIM/Politecnico di Torino labs. Two magnetizers have been designed, built, and employed for this purpose. We summarize in the following the properties of these devices, the related measuring methods, and a few significant results.

C. 2D magnetizers for high frequencies and high flux densities: design and analysis

1) The high-frequency 2D magnetizer

A two-pole three-phase machine has been designed for 2D magnetic testing up to the kilohertz range of disk-shaped samples. A 3D FEM calculation has been conducted and optimized machine geometry has been designed for an 80 mm diameter sample. The calculations take into account the specifications of the supply system, consisting of three CROWN AUDIO 5000VZ power amplifiers (peak-to-peak output voltage 300 V, maximum output current 40 A), driven by three synchronized Agilent 33220a function generators. The feedback system employed for the control of flux density loci is based on the contraction mapping principle [START_REF] Ragusa | A three-phase single sheet tester with digital control of flux loci based on the contraction mapping principle[END_REF]. The scheme of the magnetizer and the adopted 3D FEM meshing is shown in Fig. 11, together with the actual device. This is equipped with a toroidal winding, which avoids long overhangs. Three slots per pole are used, totaling 18 slots. The laminated core is made of 0.35 mm thick non-oriented Fe-Si sheets, whose experimental anhysteretic curve is taken as magnetic constitutive equation of the material in the FEM calculations. Details on the modeling criteria and procedure are discussed in [START_REF] De La Barrière | A novel magnetizer for 2D broadband characterization of steel sheets and soft magnetic composites[END_REF]. Two main points are stressed here: 1.

The disk sample is separated from the magnetizing core by a 1 mm thick gap. This narrow air gap allows to minimize the apparent power required by the magnetizer.

2.

The axial height T of the magnetizing core is optimized by 3D FEM calculations to maximize the flux density in the sample under a given magnetizing power. By taking the anhysteretic constitutive equation for a standard type of nonoriented sample of thickness d, the calculations show, in particular, that, for a ratio T/d  75, minimum apparent power is required in order to achieve a defined peak flux density value (e.g. Bp = 1.5 T at 1 kHz). For d = 0.20 mm, a 15 mm thick core is therefore predicted. For measurements performed with the fieldmetric method, a 1 mm thick 20 mm  20 mm crossed H-coil, placed in the central region of the disk sample, is employed. The capacitive effects are minimized by adequately spacing the turns, for kHz range operation. The need for open samples and the relatively small T/d ratio might have detrimental effects on the uniformity of the flux density across the measuring region. This should then be preemptively verified, as done in the present case by 3D FEM analysis. An example is here provided, where, according to Fig. 12, we take the reference axes (x, y) originating at the center of the disk sample and we regulate phase and amplitude of the magnetizing currents in such a way that unidirectional magnetization along the y-axis is obtained, averaging to Bp = 1.5 T along the 40 mm wide measuring region covered by the By = By(x, y = 0) coil. The calculated flux density By(x,y = 0), which behavior through the whole disk width is plotted in Fig. 13, turns out to be quite uniform across such a region (0.2% of relative difference). The same 3D FEM analysis was used to evaluate the uniformity of the effective magnetic field strength at the sample surface. Fig. 14 provides the behavior of Hy(x,y), paralleling the dependence of By(x, y = 0) shown in Fig. 13, on the square centered region of size 40 mm (a) and the inner square region of size 20 mm (b). The inhomogeneity of the magnetic field strength (about 31% decrease from y = 0 to y =  20 mm) with respect to the flux density is inevitably due to the strong non-linearity of the B(H) dependence at Jp = 1.5 T. In order to have good congruence between the B and H signals, a square 20 mm sized H-coil is adopted. This analysis leads to similar results and conclusions for the high-flux density 2D magnetizer, to be discussed in the following.

2) The high-flux density 2D magnetizer

In order to fully cover the aimed at (B, f) domain envisaged in Fig. 10, a novel magnetizer, specifically designed for 2D measurements at high flux densities, was developed. In such a device, the basic structure of the previous high-frequency magnetizer was retained, together with the 80 mm diameter sample. However, with the same two-pole/three-phase 18 slot configuration, re-sizing of the magnetizer was required. The thermometric measurements at high flux densities, in fact, are preferably performed under near-adiabatic conditions, which are in the present case emulated by keeping the sample inside a vacuum bell (p  10 -3 Pa), which occupies the stator bore, as sketched in Fig. 15. The 6 mm thick walls of the vacuum chamber, made of PVC, introduce a relevant airgap and the optimized T/d ratio will differ from the value found for the previous setup. An additional constraint is posed by the maximum current of 40 A per phase delivered by the CROWN AUDIO 5000VZ power amplifiers (little constraint on the voltage is posed at power frequencies). By keeping the previous winding scheme, the magnetomotive force (MMF.) per slot necessary to reach Bp = 2 T at the sample center has been computed by FEM analysis as a function of T/d [START_REF] De La Barrière | A novel magnetizer for 2D broadband characterization of steel sheets and soft magnetic composites[END_REF]. From the results shown in Fig. 16, obtained with d = 0.20 mm, the optimized value T/d = 150, that is T = 30 mm, is estimated, with the MMF. per slot around 1000 A. This condition is satisfied, taking into account the 40 A upper limit for the magnetizing current, by inserting 25 turns per slot. Assuming a maximum current density of 5 A/mm 2 (forced air convection is used to cool the windings), the geometrical parameters of teeth and back core of the magnetizer are then calculated, as summarized in Table I. To remark that the thermal transfer due to Joule heating of the windings and their forced cooling does not influence the temperature of the sample, which is protected in the vacuum chamber. As previously, stressed, the large uncertainty of the loss value measured by the conventional fieldmetric method at high flux densities can be overcome by measuring the dissipated power through the rise of the sample temperature. This can be easily detected, in particular, by a copper-constantan extended junction, carefully glued by silver paint on the sample surface, along and close to the B-windings. The reading of the junction signal is made by a calibrated nanovoltmeter, which output signal upon switch-on and switch-off of the magnetic field strength displays the typical behavior shown in Fig. 17. The magnetic field strength is applied at time ton, after stabilizing the whole device temperature, and switched off at time toff. The temperature difference between the temperature at a certain instant t and the one at time ton is called Δθ. Since the system is not fully adiabatic, we observe a typical first order system increase of Δθ vs. t till switch-off at time t = toff, followed by an exponential decrease. Consequently, [START_REF] Ferrara | Effective versus standard Epstein loss figure in Fe-Si sheets[END_REF] does not apply, but we can nevertheless precisely retrieve the power loss figure by modeling the heat exchange process according to the balance equation

         (11)
Fig. 17.: Temperature versus time in a non-oriented Fe-Si alloy subjected to rotational magnetic field strength at 20 Hz from time ton to time toff . The temperature difference Δθ(t) follows an exponential dependence on time, with time constant  = cp/Kext, where cp is the specific heat of the alloy and Kext is the heat transmission coefficient, by which we lump the imperfect adiabatic response of the sample. The continuous fitting lines are calculated from ( 12) and ( 13).

where we denote by dt dQ / in and dt dQ / out the rates at which heat is stored in the sample and lost to the environment, respectively, and by Kext the heat transmission coefficient. The increase of the specimen temperature T with time is then obtained from [START_REF] Sasaki | Measurement of rotational power losses in silicon-iron sheets using wattmeter method[END_REF]

as ext on on off 1 p 1 exp ( ) ,( ) P K t t t t t K c                          (12)
In the limit Kext  0, this equation reduces to the linear relationship [START_REF] Ferrara | Effective versus standard Epstein loss figure in Fe-Si sheets[END_REF]. The coefficient Kext is unknown, but it can be found by fitting the exponential decay of temperature observed after switch-off. If at the instant of time toff the temperature difference is Δθ1, the time dependence of the temperature difference is obtained, by posing P = 0 in [START_REF] Sasaki | Measurement of rotational power losses in silicon-iron sheets using wattmeter method[END_REF], as

  ext 1 off off p exp ( ) , K t t t t c                  (13)
We find that the temperature decay is accurately described by [START_REF] Enokizono | Rotational power loss of silicon steel sheet[END_REF], with the time constant  = cp/Kext. For the specific case of the Fe-(3.5wt%)Si sheet sample of Fig. 17, having specific heat cp = 470 Jkg -1 K -1 , we obtain from (13) the time constant  = 48.7 s and Kext = 9.65 Jkg -1 K -1 s -1 The value of P is then determined by fitting through [START_REF] Abou-Elyazied Abdallh | A Non-Destructive Methodology for Estimating the Magnetic Material Properties of an Asynchronous Motor[END_REF] the experimental Δθ vs. t increase in the time interval (toff  ton). It is noted that, by limiting the measurement to very short times (toff  ton) <<  ( = 49 s in Fig. 17) a straight line is a good approximation to [START_REF] Abou-Elyazied Abdallh | A Non-Destructive Methodology for Estimating the Magnetic Material Properties of an Asynchronous Motor[END_REF] and we can retrieve P by [START_REF] Ferrara | Effective versus standard Epstein loss figure in Fe-Si sheets[END_REF]. In the example reported in Fig. 17, we find by ( 12) P = 1.16 W/kg. The high-frequency RSST magnetizer has been used for unidirectional and 2D loss measurements up to the kHz range in steel sheets and Soft Magnetic Composites (SMC). Fig. 18 provides an example of measured alternating Walt and rotational (circular flux loci) Wrot losses in 0.20 mm thick non-oriented Fe-Si (up to 1.5 T / 2 kHz) and Fe-Co (up to 2.1 T / 5 kHz) sheets. The skin effect under alternating and circular polarization is put in evidence at the highest frequencies [90] [91]. One can notice in Fig. 18 the progressive disappearance of the maximum of Wrot vs. Jp on increasing the magnetizing frequency, a phenomenon also observed in [START_REF] Zurek | Rotational power losses and vector loci under controlled high flux density and magnetic field in electrical steel sheets[END_REF]. This behavior is understood in terms of growing share of the classical loss component in the total loss, a quantity monotonically increasing with Jp [START_REF] Appino | Alternating and Rotational Losses up to Magnetic Saturation in Non-Oriented Steel Sheets[END_REF]. Measurements of Walt and Wrot at high frequencies in SMC materials, which, because of their granular structure, are expected to bear some advantage in terms of loss behavior, are reported in Fig. 19 These samples have been obtained following different processes, leading to different average particle size and density . It is observed how the loss increases with decreasing material density (from  = 7450 kg/m 3 to  = 7110 kg/m 3 on passing from sample 1 to sample 3), that is, increasing the thickness of the intergrain boundaries. At the same time, Wrot moves its maximum value to lower Jp values. Grain decoupling, ensuing from thicker non-magnetic boundaries, yields higher coercivity (i.e. higher quasi-static losses). On the other hand , the coherent moment rotations also start at lower Jp values, because the required applied magnetic field strength, largely increased to compensate higher internal demagnetizing fields, becomes high enough to induce coherent rotations in the favored grains

The high-flux density magnetizer shown in Fig. 15 permits to approach the magnetic saturation under alternating and twodimensional magnetic field strengths in steel sheets. To this end, both fieldmetric and thermometric methods are applied upon the low-and high-flux density range, respectively. An example is provided in Fig. 21, concerning the behavior of Walt and Wrot in a non-oriented Fe-(3 wt %)Si sample, brought up to Bp = 2.0 T (Jp = 1.95 T). The fieldmetric method is applied up to about 1.6 T, the thermometric method beyond this limit, with a short overlap region. The capability of this system to measure the value of Wrot very close to the saturated state allows reaching the limiting condition, where domain walls collapse, and only coherent reversible rotations are deemed to provide the macroscopic rotation of the magnetization. In this case, the measured loss should reduce to the classical loss component, according to the equation

f B d W W    2 p 2 2 class rot, rot 3    [J/kg] ( 14
)
where  is the electrical conductivity, and d and  are the previously introduced sheet thickness and density, respectively. Using [START_REF] Zhu | Two dimensional measurement of magnetic field and core loss using a square specimen tester[END_REF] and the experimental Wrot(f) behavior at different Jp values [START_REF] Appino | Alternating and Rotational Losses up to Magnetic Saturation in Non-Oriented Steel Sheets[END_REF], we can separate Wrot(Jp) in the NO Fe-Si sheet of Fig. 21 into its hysteresis Whyst(Jp), excess Wexc(Jp), and classical Wclass(Jp) components up to saturation, as shown in Fig. 22. Here we prove that by [START_REF] Zhu | Two dimensional measurement of magnetic field and core loss using a square specimen tester[END_REF] we identify the limiting value of the rotational loss for Jp = Js. IV. CONCLUSIONS We have discussed the problems connected with the measurement of the magnetic properties of soft magnetic materials under alternating and two-dimensional magnetic field strengths and related recent advances, with a focus on recent investigations and advances obtained by the cooperative activity of the SATIE, INRIM, and Politecnico di Torino labs.

The Epstein and SST standard measuring methods and the systematic deviations of their power loss figures from the true values, follow from the specifically involved magnetic circuits and the practical need to define a magnetic path length. This, however, inevitably depends on the sample type, the flux density level, and the magnetizing frequency. Detailed analysis of the Epstein measurements made on different NO and GO Fe-Si sheets shows, for example, that in all materials the effective magnetic path length increases with the peak polarization, differing by up to about 5 % with respect to the standard 0.94 m path length [START_REF] Ferrara | Effective versus standard Epstein loss figure in Fe-Si sheets[END_REF]. A Single Sheet Tester with double-C flux-closing yoke has therefore been developed, by which the magnetic path length is independent of the material type and flux density level by means of an original compensation method, based on the use of the yoke itself as a zero-MMF indicator. Systematic deviations from the true loss values are in this way reduced to less than 1 %, that is within the typical uncertainty of this kind of measurements.

The present-day capabilities of the two-dimensional measuring systems lack in general the access to frequencies in the kHz range at technical flux densities and to high flux densities at power frequencies. But testing at high frequencies and high flux densities meets the demand by today machine designers. To overcome current limitations, the authors have developed novel setups, based on 3D FEM designed three-phase magnetizers, employed with disk-shaped samples, minimum airgap, highperformance power amplifiers, and dedicated feedback algorithms. Loss measurements up to 2 kHz at 1.5 T could be made, for example, in 0.20 mm thick non-oriented Fe-Si sheets, a range broadened to 2.1 T and 5 kHz in the high-saturation Fe-Co alloys. Soft Magnetic Composites could also be tested up to 1 kHz at 1.25 T. These figures largely exceed previous literature reports. On the other hand, the saturation magnetization could be closely approached in non-oriented Fe-Si sheets at power frequencies. It is here verified, in particular, that Wrot is reduced to the classical component, as expected on theoretical grounds, but never experimentally proved.

V. REFERENCES

[1] P. Di Barba, M. Bonislawski, R. Palka, P. Paplicki, and M. Wardach, "Design of hybrid excited synchronous machine for electrical vehicles," IEEE Transactions on Magnetics, vol. 51, no. 6, pp. 1-6, 2015.

E> 2 Fig. 1 .

 21 Fig. 1. Ratio of the Epstein to the effective ("true")power loss figure PEpst/Peff at 50 Hz measured in different types of non-oriented and grain-oriented steel sheets. Peff(Jp) is obtained by precise local measurement of magnetic field strength and flux density.

Fig. 2 .

 2 Fig.2. Dispersion around the reference value of the laboratories best estimate of the power loss measured by the Epstein (PEpst) and the SST (PSST) methods in GO sheets. The related intercomparison is discussed in[START_REF] Appino | International comparison on SST and Epstein measurements in grain-oriented Fe-Si sheet steel[END_REF]. N() is the number of laboratories whose best estimate Pi deviates from the reference value <P> by the relative quantity  = (Pi -<P>)/ <P>. The dashed lines are best fits of the experimental distribution by a Gaussian function. The relative standard deviation  associated with the measurements is lower than 1 %.

Fig. 4 .

 4 Fig. 4. Reduced value Jp(x) / Jp(0) of the peak polarization in NO Fe-Si strip samples across the limb length l0 = 195 mm (the length covered by the windings, with center at x = 0) of a standard Epstein frame. Jp(x) is measured by means of a localized pickup coil, collinear with a narrow H-coil, allowing for simultaneous measurement of PEpst and the local power loss Peff(x) [10].

Fig. 6 .

 6 Fig. 6. a) Compensated permeameter with upper yoke working as zero MMF indicator and the related control loop. b) Equivalent reluctance scheme.

  S (mVA/kg) J p (T)

Fig. 8 .

 8 Fig. 8. Example of Vertical Rotational Single Sheet Tester [54].

>Fig. 9 .

 9 Fig. 9. Arrangement of H-and B-windings for the 2D characterization of magnetic sheets. a) Crossed H-coils for the measurement of (dHx/dt, dHy/dt); b) Crossed B-windings, made of few turns threaded through small holes, providing (dBx/dt, dBy/dt); c) Final arrangement of the H-and B-coils for the fieldmetric measurement of 2D hysteresis loops and losses.

  we define by x and y the reference axes on the sample plane, the associated (Hx, Hy) magnetic field strength components are thus determined by means of a couple of crossed multiturn flat H-coils or by crossed Chattock coils [71] [72]. The two > FOR CONFERENCE-RELATED PAPERS, REPLACE THIS LINE WITH YOUR SESSION NUMBER, E.G., AB-02 (DOUBLE-CLICK HERE) < 10 orthogonal H-windings are wound on a rigid thin (d  1 mm) epoxy plate, as shown in Fig. 9a. The induced voltages VHx and VHy are linked to the magnetic field strength through the equations

Fig. 10 .

 10 Fig.10. Basic 2D measuring capabilities on non-oriented steel sheets by international laboratories are summarized in the Bp vs. frequency plane. The dashed line defines the enhanced upper limit jointly achieved by INRIM/SATIE/Politecnico di Torino.

Fig. 11 .

 11 Fig. 11. Three phase magnetizer designed for 2D magnetic measurements up to the kHz range. a) Schematic view and 3D FEM model. b) Assembled setup with test sample (adapted from [89]).

Fig. 12 .

 12 Fig. 12. An axis system x-y is defined on the sample surface. The three-phase currents are set in such a way that an alternating flux density of peak value Bp = 1.5 T is established along the y axis. The shadowed 20 mm square region centered on the sample surface is the H-coil zone.

Fig. 13 .Fig. 14 :

 1314 Fig. 13. Behavior of the magnetic flux density By(x, y = 0) across the 80 mm x-diameter of the non-oriented Fe-Si disk sample calculated for alternating magnetic field strength directed along the y-diameter. The B-measuring region is restricted to the -20 mm  x  20 mm region. The relative difference between By(0,0) and By(20 mm,0) is equal to 0.2%.

Fig. 15 .

 15 Fig. 15. Front and cross-sectional views of the high-flux density magnetizer. It holds the vacuum chamber employed for emulating quasiadiabatic conditions during the measurement of the magnetic power loss with the thermometric method.

Fig. 16 .

 16 Fig. 16. Magnetomotive force per slot required to reach Bp = 2 T at the center of the 0.20 mm thick disk sample as a function of the ratio T/d between axial height of the magnetizer and sample thickness.

>Fig. 18 .Fig. 19 .

 1819 Fig. 18. Alternating Walt and rotational Wrot energy losses measured with the use of the high-frequency RSST magnetizer in Fe-Si (a) and Fe-Co (b) non-oriented steels sheets up to the kHz range.

Fig. 20 .

 20 Fig. 20. Alternating Walt and rotational Wrot energy loss measured at 50 Hz in three different types of Fe-based Soft Magnetic Composites. They are subjected to different preparation treatments, leading to different mass densities . They attain the values: 1 = 7450 kg/m 3 , 2 = 7260 kg/m 3 , 3 = 7110 kg/m 3 .

  . The 80 mm diameter tested SMC disks have a thickness of 3 mm. Because of their low permeability (r  100 -500) and bulk shape, these materials pose a challenge to their 2D characterization at medium-to-high flux densities and frequency values in the kHz range. The domain (f, Jp) accessible to measurements can be roughly identified with the area subtended by the experimental limiting f(Jp) line shown in the inset of Fig. 19. This measuring capability is superior to the state of the art [92]. Typical behaviors at 50 Hz (i.e., close to quasi-static excitation) of Walt and Wrot versus Jp in different types of SMC are shown in Fig 20.

Fig. 21 .

 21 Fig. 21. Alternating Walt and rotational Wrot energy losses in NO Fe-Si sheets measured at 50 Hz up to peak flux density Bp = 2.0 T (Jp = 1.95 T).

Fig. 22 .

 22 Fig. 22. Loss separation under rotating flux density up to Jp = 0.97JS in a 0.356 thick NO Fe-Si sheet.

TABLE I

 I

	GEOMETRICAL PARAMETERS OF THE MAGNETIZER DESIGNED FOR MEASUREMENTS AT HIGH FLUX DENSITIES
	Parameter	Symbol	Value
	Sample diameter	D	80 mm
	Airgap thickness	a	6 mm
	Magnetizer axial thickness	T	30 mm
	Teeth depth	tS	45 mm
	Teeth width	wS	15 mm
	Yoke thickness	tY	20 mm
	Number of turns per coil	N	25

  > FOR CONFERENCE-RELATED PAPERS, REPLACE THIS LINE WITH YOUR SESSION NUMBER, E.G., AB-02 (DOUBLE-CLICK HERE) <

													16
	P	in dQ dt	out dQ dt	p c	d	dt	K	ext	,		t t	on	